Assembly of dye sensitized solar cell using the stem and grain
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201313Assembly of Dye-Sensitized Solar Cell using the Stem and Grainof Sorghum Bicolor as SensitizersAkingbade Fatai1, Boyo Adenike 2*, Oluwole Surukite3Abudusalami Ibrahim41,2Department of Physics, Lagos state university, Ojo, Lagos, Nigeria3Department of Botany, Lagos state university, Ojo, Lagos, Nigeria4Department of Chemistry, Fountain University, Oshogbo, Lagos, Nigeria*Email Corresponding author: firstname.lastname@example.orgAbstractRed anthocyanins from sample A (stem of sorghum bicolor) and sample B (grains of sorghum bicolor) wereemployed as TiO2 dye – sensitizers. Solar cells sensitized by the extracts of sample A achieved the following foroutdoor measurement; ISC = 0.0023mA/cm2, VOC = 0.0022V,Pmax = 3.666mV/cm2, FF = 0.7212, η= 1.7554 and for sample B outdoor measurement FF = 0.7961, Isc =0.00178mA/cm2, Voc = 0.0014V, Pmax = 4.96 x 10-6mw/cm2and η = 4.221 under the illumination of solar energy4.7x10-3W/cm2respectively. The indoor measurement values for the same dyes sensitized cells determined forsample A are ISC=0.0182mA/cm2, VOC = 0.004 V;Pmax = 3.299 x 10-7mW/cm2, FF = 0.4512, η =0.15 and sample B achieved ISC = 0.01378 mA/cm2; VOC = 0.005V, Pmax = 3.5 x 10-7mW/cm2, FF = 0.5511and η =0.18 respectively.The results show that Sample B (indoor and outdoor measurement) has higher efficiency than sample A. This isdue to the constituent of the extract .Sample A and B show a successful conversion of visible light intoelectricity by using natural dyes as band-gap semiconductor sensitizer in dye-sensitized solar cells .This can beuse in large scale to reduce power and energy requirements for future industry designs.Key Word: Sorghum Bicolor, Dye-sensitized solar cell, Solar light energy conversion, TiO21. IntroductionOne of the biggest challenges ahead of human kind is to replace the fossil fuel with renewable energy sourceswhile keeping pace with the worldwide increasing thirst for energy because of the increasing population andrising demand from developing countries. This challenge has to be answered with a low-cost solution usingabundantly locally available raw materials. The sun is an obvious source of clean and cheap energy, already usedby nature to sustain almost all life on earth. Therefore, harnessing the power of the sun with the photovoltaictechnologies appears to be the only reasonable large scale answer to the energy challenge ( Hara et al 2003).Presently, the world energy consumption is 10Tetrawatts (TW) per year, and by 2050, it is projected to be about30TW. The world will need about 20TW of non-CO2 energy to stabilize CO2 in the atmosphere by mid- century.The simplest scenario to stabilize CO2 by mid-century is one in which photovoltaic (PV) and other renewable areused for electricity (10TW), hydrogen for transportation (10TW) and fossil fuel for residential and industrialheating (10TW) (Zweibel, 2005).Thus, PV will play a significant role in meeting the world future energydemand. Among varieties of renewable energy sources in progress is the solar cell. This means harvestingenergy directly from the sunlight using photovoltaic. The solar cells that have recorded the highest photon toconversion efficiency are the first generation devices based on single silicon crystal (Belfar and Mostefaoui,2011). The problem with this solar cell is their high cost production and installation. Various researchers (Konanet al, 2007, Bhatti et al, 2012) have work on second generation devices consisting of semiconductor thin film, inorder to reduce the high cost of production and improve the efficiency of first generation solar cells, although theefficiency challenges has not been removed. The third generation solar cells are the dye sensitized solar cells,heterojunction cells and organic cells. These are similar to plants that used photosynthesis to absorb energy fromsunlight (Zainudin et al 2011; Efurumibe et al, 2012). DSSCs use dyes or sensitizers” to convert sunlight intoelectricity (Gratzel et al 2003).This study therefore intends to extract natural dye from the stem and grains of sorghum bicolor. Also toinvestigate the performance of solar cells fabricated using stems and the grains of sorghum bicolor as a sensitizerto convert solar energy into electricity. Sorghum bicolor is perhaps the world’s most versatile crop and grownacross West Africa. This plant belongs to the family of proaceae .It is called Poroporo ,Oka-baaba in Yoruba,Kaara - Daawa in Hausa and Okri in Igbo . Sorghum plays an important role as a food security crop especially insemi arid lands of Kenya. It can survive drought conditions for some weeks by rolling up its leaves and thisdecreasing transpiration. The whole plant is often used as windbreaks, forage, hay, or silage. Their stems areused for building, fencing, weaving, broom making and firewood. The seeds are fed to poultry, cattle and swine(Tsuborama et al 1976). Figure 1 illustrates the physical appearance of this wonderful plant and its grain:
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201314Fig. 1: Physical appearance of sorghum bicolor plant2.0 Structure of Dye Sensitized Solar CellThe main parts of single junction dye sensitized solar cell are illustrated schematically in figure 2 The cell iscomposed of four elements, namely, the transparent conducting and counter conducting electrodes, the nano-structured wide band gap semiconducting layer, the dye molecules (sensitizer), and the electrolyte. Thetransparent conducting electrode and the counter electrode are coated with thin conductive and transparent filmsuch as fluorine-doped tin dioxide (SnO2) (Gratzel et al 2005). The figure 3 below illustrate the red dye adsorbedonto a titanium dioxide surface (Martinson et al. 2008)Figure 2:Schematic of the structure of the dye sensitized solar cell.
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201315Fig. 3 : Red dye absorbed on a titanium dioxide surface3. 0 Method of ExtractionThe stem and grains of sorghum bicolor were purchased from Lusada market, Igbesa in Ado- Odo/Ota OgunState. Cold extraction method was used to extract the dye from sample A and B. This method was employedbecause distillation is possible at lower temperature and possibility of re-using solvent used for the extraction.50g of the stem of sorghum bicolor labeled sample A and the grains of sorghum bicolor labeled sample B eachwere weighed using OHAUS Electronic weighing balance model brain weight B1500 made in USA and crushedwith blender in order to increase the surface area of the samples to enhance speedy extraction.Each of the crushed samples were soaked in acidified 490cm3of methanol (CH3OH) i.e. 1% of 1Molar solutionof HCL was added to 490 cm3of methanol in separate covered bottles and placed inside SLAUART SSL1ORBITAL SHAKER at 25rpm for 12hours. The mixtures were allowed to stay for another 12hours which madethe soaking period to be 24hours.The extract of each of the samples were decanted to remove the residual part of the samples.Simple distillation was carried out at 650C i.e. the boiling point of methanol in order to concentrate the dye of thesamples.This distillation process is necessary for the following reasons:- To increase the concentration of the dyes- To recover part of the solvent i.e. Methanol used for the extraction in its pure state which can still be re-used.3.1.1 Measurement OF SAMPLE A AND SAMPLE B EXRACT (DYE) OF pHThe measurement of the pH of the sample’s extracts were carried out with JENWAY 3505 PH meter , PH 7.47was obtained for the extract of sample A and PH 5.14 was obtained for the extract of sample B . These valuesare known as samples pH.1.0ml from extract of sample A and B were measured and diluted with methanol to obtained PH 3.0 and 1 .0respectively. Magnetic stirrer was used to enhance thorough mixing of the dilution.3.1.2 Spectrophotometer AnalysisSpectrophotometer analysis of the extracts of sample A at the pH 7.47, 3.0 and 1.0 and sample B at the pH5.14, 3.0 and 1.0 were carried out using SURGISPEC SM-23D surgifield medical spectrophotometer at therange of frequencies 350 to 1000nm which corresponds to the frequencies of visible light spectrum to obtainedabsorption rate of the extract . In order to have the absorption of the samples with TiO2, 3ml of HNO3 + 1ml ofdye (either extract of sample A or B) + 1g of TiO2 are taken. Also, Spectrophotometer measurement of 1g ofTiO2 + 3ml of HNO3 was done. The corresponding absorbance -wavelength characteristics for all extract areshown in the figure 4 -9, absorption of the extract with TiO2 is shown in figure 10 -12.
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 2013163.1.3 Fabrication Procedure OF Dye-Sensitized Solar Cell.The TiO2 solution (paste) was prepared by the incremental addition of 20ml of nitric acid solution to 20g ofcolloidal TiO2 powder in a mortar and pestle while grinding for about 20minutes to enhance a uniform and lump-free paste.A digital multimeter was used to check which side of the FTO glass purchased from HARTFORD GLASSCOMPANY USA is conductive and the reading was 32.0 Ω.Adhesive –tape are applied to the face of the conductive glass plate in order to create on opening of dimension1.5 x 1.5cm2at the centre of the glass. This tape formed about 40µm deep mold into which the TiO2 solution canflow and at the same time masks a strip of the conductive glass so that an electrical contact can later be made.Three drops of TiO2 paste was dropped at one edge of the opening and spread uniformly using glass rod. Thefilm was then allowed to dry in air for 1minute. The tape was then carefully removed and the film was annealedand sintered in an oven at 100oC for 20 minutes. The TiO2 –coated conductive glass was allowed to slowly coolto room temperature. The prepared TiO2- coated conductive glass which is called TiO2 electrode was dipped intothe dyes solutions for 10minutes. It was then taken out from the dye solution and washed with fresh methanoland allowed to dry for another 5minutes3.1.4 Preparation of Counter ElectrodeThe counter electrode was prepared using a conductive glass of dimension 2.5x7.5cm purchased fromHARTFORD GLASS COMPANY USA.The conductive surface of the glass was coated with carbon generated form candle flame. This serve as catalystfor the tri-oxide to iodide generation reaction .This electrode prepared is known as positive electrode (Anode).The stained dried electrode (cathode) was then placed on the table such that the film side faced up, and thecatalyst- coated electrode (anode) was placed on the top so that the conductive side of the counter electrode facesthe TiO2 film. The two opposing glass plates are offset so that all of the TiO2 is covered by the counter electrodeand the strip of the glass not coated by TiO2 was exposed. The two exposed sides of the glasses serve as cathodeand anode respectively. Two binder clips were used to gently hold the plates together at the other edges. Twodrops of iodide electrolyte solution of 0.5M was then placed at the edges of the plates binder clips arealternatively opened and closed while in place. The electrolyte was drawn into the place between the electrodesby capillary action and in order to wet stained TiO2 film.3.1.5 Measurement of Photoelectric Conversion efficiency of the DSSCThe completed solar cell was then taken outside under the illumination of sunlight to obtain the outdoormeasurement for current and Voltage. A 50W, 12V halogen lamp manufactured by GE lighting, LLC Nela parkassembled in USA was used obtain indoor measurement for current and Voltage using sorghum bicolor solarcell. Solar energy conversion efficiency (the photocurrent -voltage) was measured by using digital multimetersunder the illumination of sunlight and 50W halogen lamp. The active area of the cell is 1.5 × 1.5 cm2.The cicuitdiagram of the cells for the measurement of I – V is shown in the figure 4.Figure 4: Circuit diagram for solar cells measurement
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 2013174.0 Results and DiscussionThe figures 5-10 shows the acquired absorption spectra at the wavelength 350 – 1000nm of visible lightspectrum for extract (dye) of sample A and sample B .we observed that only the extract (dye) of sample Aaccording to figure 6 gives better absorption of 220 at wavelength 500nm which falls within the range of 400nmto 800nm parts of electromagnetic spectrum.Extract (dye) of sample B also show absorption values of 1.488, 5.3 and 3.0 respectively at wavelength of350nm which does not fall within the range of visible part of electromagnetic spectrum.Absorption – wavelength characteristics of 1ml of extract (dye) of sample A and sample B mixed with threemills of HNO3 on 1g of TiO2 at the wavelength of 350 – 1000nm respectively are plotted in figure 11 – 13Better absorption of visible part of electromagnetic spectrum was obtained with extract of Sample A. TiO2 alsoshowed a reasonable absorbance with HNO3 at PH 1.00.It therefore showed that the extract of sample Aabsorbed visible part of electromagnetic spectrum than extract of sample B despite the fact that both samples arefrom the same source. This is due to the structure of the sample B extract resulting in a stronger steric hindrancefor anthocyanin to form bond with oxide surface and prevents the anthocyanin molecules from arranging on theTiO2 film effectively (Mor et al, 2006). Hence, this leads to a deficiency of electron transfer from the dyemolecules in the conducting band of TiO2 (Boyo et. al 2012).Figures 14-17 is the photovoltaic performances that were obtained with a sandwich cell under illumination bysimulated solar light (outdoor measurement) and 50W halogen lamp (indoor measurement). The photocurrent –voltage curves of the assembled solar cells are used to evaluate the cells performance.Table 1 – 2 show the photo electrochemical parameters of the cells sensitized with natural extracts (dyes) ofsample A and B for outdoor measurement and indoor measurement respectively. It was observed that theefficiency of cells assembled with extract of sample B is of greater value than sample A for the indoormeasurement and outdoor measurement as shown in the tables 1-2. This shows that sample B has ability ofharvesting solar energy than sample A5.0 ConclusionSuccessful conversion of visible light into electricity was achieved by red anthocyanins from the extracts ofsample A and sample B as TiO2 dye-sensitizers. The anthocyanins present in the extracts are capable to bechemically absorbed onto the semi-conductor surface, sensitizing it to the visible region of the spectrum eventhough extract of sample A has low absorption values. The energy of the dye excited state is also appropriate topromote the electron injection into the semiconducting band, consequently, converting the sunlight into electricaloutput. Therefore the use of natural dyes can be an alternative for a lower cost production of dye-sensitized solarcells, being environmentally friendly, renewable and clean source of energy. It is also useful to demonstrateseveral important scientific concepts (materials, semiconductors, molecules devices etc.) for educationalpurposes.REFERENCESBelfar, A. and Mostefaoui (2011). Simulation of n1 – n2 microcrstalline silicon tunnel junction with AMPS – IDin a Si: H/NC – Si: tandem solar cells. Journal of applied science, 11: 2932 – 2939Bhatti, M. T., Rana, A .F. Khan and Ansarfi M. I (2012). Effect of annealing on electrical properties of indiumTin Oxide (ITO) Thin Films. Journal of applied science, Volume 2, 570-573Boyo A. O. Boyo H. O Shitta M.B.A, Abdusalam I., Fajana O.O and Awodibo M.A (2012). Fabrication of Dye- solar cells (DSSC) device using lawsonia intermis leaf, international Journal of pure and applied physics,Volume 8, Number 2 , 59 - 68.Efurfumibe, E.L., Asisgbu, A.D. and Onuu, M.U. (2012). Mathematical modeling of electron transport throughthe anode (TiO2) of a standard dye sensitized solar cells. Asian Journal of applied science volume 5, 34 - 42.Gratzel, M. (2003). Dye-sensitized solar cells. Journal of photochemical and photobiology C. Photochemistryreview 4, 145 -153Gratzel, M. (2005). Solar energy conversion by Dye-sensitized photovoltaic cells. In org. Chem, Vol. 44 pp.6841 – 6851Hara, K. and Arakawa, H. (2003). Dye-sensitized solar cells, In: Handbook of photovoltaic science andEngineering, A. Luque ad s. Hegedus, (Ed); Chapter 15, pp. 663 – 700, John Wiley and Sous, LTd, ISBN: 0 –471 – 49196 – 9.
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201318Konan K. Soraka, J.K., Zouneu, J.I and Gbaha P., (2007). Structure and morphological analysis of CuInse2 thinfilms prepared by vaccum free CSVT for photovoltaics cells. Journal of applied science volume 7,478 - 483.Martinson, A. B. F., hamann, T.W., Pellin, M.J, and Hupp, J.T., (2008). New architectures for dye-sensitizedsolar cells. Chemistry - Eur. Journal, Volume 14, 44578 – 4467.Mor, G. K; Shanker, K., Paulose, M; varghedse, O.K and Grimes, C.A (2006). Use of highly ordered TiO2nanotube Arrays in Dye- sensitized solar cells. Nonaletters, volume 6, issue 2, 215 – 218.Tsuborama, H., Matsumura, M., Nomura, Y., Amamiya, T. (1976) Nature 261, 402.Zainudin, S.N.F., Markom, H. Abdulah, R., Adami and Tasirm, S.A (2011). Supercritical anti - solvent processfor enhancement of dye – sanitized solar cell efficiency: A review , ASIAN. J. Applied sci., volume 41. 331 –342.Zweibeli K. and gree, M.A. (ed) (2005). Progress in photovoltaics research and application volume 8, issue I,171 – 185.Fig.5: Light absorption spectra of Extract (dye) of sample A at PH 7.47Fig. 6: Light absorption spectra of Extract (dye) of sample A at PH 3.000.2820.2840.2860.2880.28100.28120.28140.28160.28180.28350 450 550 650 750 850 950ABSORBANCE(AB)WAVELENGHT λ (nm)-50050100150200250300350 450 550 650 750 850 950ABSORBTION(AB)WAVELENGHT λ ( nm)
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201319Fig. 7: Light absorption spectra of Extract (dye) of sample A at PH 1.00Fig8: Light absorption spectra of Extract (dye) of sample B at PH 5-50050100150200250350 450 550 650 750 850 950ABSORBTION(AB)WAVELENGHT λ (nm)-0.0120.4880.9881.4881.9882.4882.9883.4883.9884.488350 450 550 650 750 850 950ABSORBTION(AB)WAVELENGHT λ (nm)
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201320Fig. 9: Light absorption spectra of Extract (dye) of sample Bat PH 3.00Fig. 10: Light absorption spectra of Extract (dye) of sample B at PH 1.000123456350 450 550 650 750 850 950ABSORBANCE(AB)WAVELENGHT λ (nm)00.511.522.533.5350 450 550 650 750 850 950ABSORBTION(AB)WAVELENGHT λ (nm)
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201321Fig. 11: Light absorption spectra of 1ml of extract (dye ) of sample A + 3ml of HNO3 on 1g of TiO2.Fig. 12: Light absorption spectra of 1ml of extract (dye) of sample B + 3ml of HNO3 on 1g of TiO2.00.20.40.60.8188.8.131.5250 450 550 650 750 850 950ABSORBANCE(AB)WAVELENGHT λ ( nm)00.20.40.60.8184.108.40.206.8350 450 550 650 750 850 950ABSORBANCE(AB)WAVELENGHT λ (nm)
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201322Fig.13: Light absorption spectra of 3ml of HNO3 on 1g of TiO2.Fig. 14: I-V curve for sample A extract sensitized solar cell of 1.5 × 1.5 square centimeter (outdoormeasurement).00.20.40.60.811.2350 450 550 650 750 850 950ABSORBANCE(AB)WAVELENGHT λ (nm)01234560 0.5 1 1.5 2 2.5Cellcurent,I(mA)x10-3Cell voltage,V(mV)
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201323Fig. 15: I-V curve for sample B extract sensitized solar cell of 1.5 × 1.5 square centimeter (outdoormeasurement).Fig. 16: I-V curve for sample A extract sensitized solar cell of 1.5 × 1.5 square centimeter (outdoormeasurement).00.511.522.533.544.50 0.5 1 1.5Cellcurrent,X10-3(mA)Cell voltage, V(mV)00.511.522.533.544.50 0.01 0.02 0.03 0.04 0.05CellCurrentI,x10-2(mA)Cell Voltage,V (mV)
Journal of Natural Sciences Research www.iiste.orgISSN 2224-3186 (Paper) ISSN 2225-0921 (Online)Vol.3, No.5, 201324Fig.17: I-V curve for sample B extract sensitized solar cell of 1.5 × 1.5 square centimeter (outdoormeasurement).Table 1.Outdoor Measurement for cells of sample A and BExtracting Solvent Extract Voc (mV) ISC (mA/cm2) η% FFCold extraction Method Sample A 220 0.00023 1.7554 0.7212Cold extraction Method Sample B 140 0.00178 1.891 0.7961Table 2.Indoor Measurement for cells of sample A and BExtracting Solvent Extract Voc (mV) ISC (mA/cm2) η% FFCold extraction Method Sample A 40 0.0182 1.4799 0.4512Cold extraction Method Sample B 50 0.01378 1.7554 0.5511000.511.522.533.50 0.001 0.002 0.003 0.004 0.005 0.006CellCurrentI,10x-2(mA)Cell Voltage, V (mV)
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar